PHYSICAL REVIEW LETTERS

week ending 31 JANUARY 2014

Localized Orientational Order Chaperones the Nucleation of Rotator Phases in Hard Polyhedral Particles Vikram Thapar and Fernando A. Escobedo,* School of Chemical and Biomolecular Engineering, Cornell University, Ithaca, New York 14853, USA (Received 26 July 2013; revised manuscript received 8 November 2013; published 28 January 2014) The nucleation kinetics of the rotator phase in hard cuboctahedra, truncated octahedra, and rhombic dodecahedra is simulated via a combination of forward flux sampling and umbrella sampling. For comparable degrees of supersaturation, the polyhedra are found to have significantly lower free-energy barriers and faster nucleation rates than hard spheres. This difference primarily stems from localized orientational ordering, which steers polyhedral particles to pack more efficiently. Orientational order hence fosters here the growth of orientationally disordered nuclei. DOI: 10.1103/PhysRevLett.112.048301

PACS numbers: 82.70.Dd, 47.57.J-, 81.10.Aj, 83.10.Rs

Homogeneous nucleation is the key step in spontaneous crystallization in which an embryo of a stable solid phase is created within a metastable liquid. Understanding nucleation remains a challenge, as it is an activated process that involves overcoming a free-energy barrier by a rare fluctuation in the metastable phase. Conceptually, classical nucleation theory (CNT) [1] is widely used to provide a framework to study nucleation kinetics. CNT assumes that each nucleus is spherical and formed by the single most thermodynamically stable solid; the size of the largest nucleus serves as the only relevant order parameter to monitor the kinetics of the process whose transition state defines the critical nucleus size. Although useful, this simplified picture has also proven to be incomplete. For Lennard-Jones spheres, e.g., the shape and structure of the critical nuclei are important to describe the nucleation mechanism [2]. Molecular simulations provide a more rigorous tool to probe the mechanism of nucleation. However, conventional brute force simulations are impractical as nucleation is a rare event, which makes it difficult to collect enough statistics with computing resources typically available. To overcome this limitation, many sophisticated methodologies have been developed [3–12]. Among them, forward flux sampling (FFS) [11,12] is particularly appealing given its ability to simultaneously and efficiently resolve the transition path ensemble (TPE), the committor probabilities, the transition state ensemble (TSE), and the transition rates. FFS generates the TPE by “ratcheting” partial trajectories forward (and over large free-energy barriers) by the use of interfaces placed along an order parameter that tracks the phase space between the two basins of interest. Despite the multiple simulation studies and different techniques that have been used to examine nucleation processes, most of them have been concerned with spherical particles given their simplicity and relevance to some atomic and colloidal systems. At present, however, a major focus in material science is the self-assembly of anisotropic 0031-9007=14=112(4)=048301(5)

particles due to its potential to help engineer novel materials from colloidal nanoparticles [13,14]. Assemblies of anisotropic particles undergo order-disorder phase transitions involving changes in both translational and orientational degrees of freedom and can lead to phases with partial structural order or “mesophases” [15]. Recent studies [16–19] have provided a partial road map of the mesophases that can be expected for different types of polyhedral particles. Along with the phase behavior, understanding the kinetics of the phase transition of anisotropic particles is also of practical importance (e.g., kinetic traps may preclude the timely formation of a desirable phase) and yet this has been either scantly explored (for rodlike particles) [20–23] or completely unexplored (for polyhedral particles). In this work, we focus on the rotator-phase nucleation in hard cuboctahedra (CO), truncated octahedra (TO), and rhombic dodecahedra (RD). They are representative of a class of polyhedral particles that form crystals with welldefined translational and orientational order at high concentrations [16,18,19]. At the order-disorder transition pressure, the isotropic phase of suspensions of these polyhedra transitions into a rotator or plastic mesophase wherein particles are translationally ordered but essentially orientationally disordered. Given that primarily translational order is nucleated, one could conjecture that the kinetics of the rotator-phase nucleation of COs, TOs, and RDs is comparable to that for the nucleation of translational order in suspensions of hard spheres (HSs). This is particularly relevant in comparing COs and HSs since, as it is shown in the Supplemental Material [24], the rotator phase in COs has (unlike those for TOs and RDs) minimal long-range orientational order at all pressures where it is stable. We show here that the above conjecture of kinetic similarity is incorrect. We find that while the size and shape of the subcritical and critical solid nuclei do bear similarities to those seen in HSs, for COs, TOs, and RDs the freeenergy barrier is significantly lower, and the nucleation rate is significantly faster than those in HSs for comparable

048301-1

© 2014 American Physical Society

week ending 31 JANUARY 2014

PHYSICAL REVIEW LETTERS

PRL 112, 048301 (2014)

Table I. Simulation data for the rotator-phase nucleation in COs, TOs, and RDs. ηliquid is the liquid phase packing fraction at pressure P . ΔG =kB T is the free-energy barrier height and ntr is the critical cluster size. Shape CO CO CO TO TO TO RD RD RD

P

ηliquid

DSS

Iσ 5 =D0

ΔG =kB T

ntr

4.1 4.6 4.8 2.8 3.0 3.15 4.32 4.56 4.64

0.513 0.529 0.532 0.496 0.504 0.5085 0.5008 0.5072 0.511

0.30 0.38 0.44 0.30 0.42 0.52 0.34 0.44 0.51

ð1.9 0.5Þ × 10−14 ð2.0 0.6Þ × 10−08 ð1.0 0.5Þ × 10−6 ð1.0 0.5Þ × 10−12 ð5.8 0.8Þ × 10−07 ð1.8 0.7Þ × 10−05 ð3.2 1.3Þ × 10−09 ð3.0 0.5Þ × 10−06 ð1.6 0.5Þ × 10−05

19.8 0.8 3.4 0.2 2.5 0.3 18.5 0.7 4.9 0.2 1.7 0.1 10.9 0.6 3.2 0.1 1.9 0.1

177 55 31 165 59 29 117 40 25

degrees of supersaturation. We identify small regions of spatially correlated orientationally and translationally ordered particles likely acting as a catalyst for the rotator-phase nucleation in the polyhedra (such regions are local fluctuations that foreshadow the establishment of long-range orientational order to ensue at higher pressures). FFS has been used to study the crystal nucleation in various systems [25–27]. From the FFS variants available, we apply here the constrained branched growth algorithm [28–31], as it has been shown to be efficient and to allow a cost-free estimation of committor probabilities (pB ) [31]. To estimate the nucleation free-energies, we have used a multiple-window umbrella sampling (US) method [29,30]. We use the number of particles in the largest (translationally ordered) solid cluster, ntr , as a reaction coordinate. To estimate ntr , we adopted the order parameter introduced by ten Wolde et al. [5] to distinguish between liquidlike and solidlike particles as pertaining to the mesophases that the polyhedra form. Details on the calculation of ntr and transition rates are provided in [24]. The simulations were conducted in a cubic cell with periodic boundary conditions, with fixed number of particles, N (¼ 3375 for COs, 2500 for TOs, and 2916 for RDs), and constant reduced pressure P ¼ βPσ 3 =8, where σ; is the diameter of the circumscribing sphere (specific to each particle geometry) and β ¼ 1=kB T. P values are chosen such that the degree of supersaturation (DSS) approaches the range of values for which nucleation studies for HSs have been performed. The DSS is calculated via [32]: DSS ¼ βjΔμj;

(ii) 0.3 and 0.42 for TOs, and (iii) 0.34 and 0.44 for RDs, while we used a brute force approach similar to that used in Ref. [33] for the largest DSS for all shapes. We used kinetic Monte Carlo (KMC) simulations to evolve trajectories from liquid to solid as in Refs. [34–35]; further simulation details are given in [24]. Table 1 shows the calculated nucleation rates for COs, TOs, and RDs. The nucleation rate, I is given by I ¼ ðT AB VÞ−1 , where V is the volume of the system and T AB is the mean first passage time from the liquid basin to the rotator basin. Rates are given in dimensionless form I ¼ Iσ 5 =D0 , where D0 is the free-particle diffusion constant (see Ref. [34,35] for details) and is assumed to be comparable for all four shapes. In Fig. 1(a), we show the free-energy profile over ntr obtained from US. In Table 1 and Fig. 1(b) we compare the nucleation rate and freeenergy barrier height ΔG among HSs, COs, TOs, and RDs. As expected, I increases and ΔG decreases with DSS for all shapes. Our results also show that for all three polyhedra ΔG is significantly smaller and I significantly larger than those for HSs. This is intriguing considering that all these hard-particle systems (HSs and COs in particular) could be thought of as cases where a similar translationally ordered, rotationally disordered phase is being nucleated. To find some clues to explain such disparity, we proceed to

(1)

where jΔμj is the chemical potential difference between the metastable fluid and the stable solid at the simulated P , obtained using thermodynamic integration (see [24]). jΔμj embodies the true thermodynamic force driving the nucleation of the new phase. The values of P and DSS are given in Table 1. DSS values > 0.55 were not explored since the liquid phase would become unstable. We performed FFS calculations at DSS values of (i) 0.3 and 0.38 for COs,

DSS

FIG. 1 (color online). (a) Free-energy profile Gðntr Þ=kB T as a function of ntr , and (b) Free-energy barrier height ΔG =kB T and nucleation rate, I vs DSS ¼ βjΔμj for COs, TOs, and RDs. HS data from [36].

048301-2

PRL 112, 048301 (2014)

PHYSICAL REVIEW LETTERS

examine the microstructure of the nuclei using the configurations collected at different FFS interfaces. First we note that, like in HSs, the growing nucleus in the polyhedra tends to have a spherical shape (see [24]). To characterize translational order, we calculate f α , the fraction of crystal structure type α in such a nucleus (see also [24] for details). Figure 2(a) shows the results of f α as a function of ntr for COs, TOs, and RDs. Similar to HSs [30,32], the small clusters for the polyhedra have some bccand liquidlike signatures, but unlike HSs [36], the most dominant structure is hcp with a very small contribution of fcc. The dominance of hcp-like motifs for COs and TOs is likely a reflection of the stable structure of their plastic solids: hcp for COs and bct for TOs [18]. The prevalence of hcp motifs in the critical nucleus for RDs rather than the bulk-solid fcc structure can be seen as a manifestation of Ostwald “step rule.” A lower free-energy barrier may be the result of nucleating hcp-like clusters in the polyhedra rather than fcc-like clusters in HSs. However, it seems unlikely that the small structural dissimilarity between hcp and fcc lattices is the sole reason for the much lower nucleation free energy barriers in the polyhedra. To quantify orientational order, we use parameters P4 and I 4 [24,37], which capture any trace of the cubic orientation symmetry that COs, TOs, and RDs will fully attain in the crystalline state. In accord to previous observations [16,17], particles in the bulk rotator phases of these polyhedra near the isotropic-rotator coexistence pressure dynamically rotate (with liquidlike rotational diffusivity) in all possible directions, but do have a small amount of long-range orientational order. This is a reflection that particles are trapped in (translationally ordered) “cages” that are not perfectly spherical. We show in the Supplemental Material [24] that, for the COs in particular, the extent of long-range orientational order is small enough for the rotator phase to be considered orientationally disordered at any of the pressures investigated. As it turned

FIG. 2 (color online). Translational and orientational order in solid nuclei of COs, TOs, and RDs. (a) Relative weight of the structural signatures for bcc, fcc, hcp, and liquidlike ordering. (b) Variation of PCl 4 with ntr ; P4 values for ntr ¼ N correspond to the bulk rotator phases, and P4 for the liquid phase is shown as a horizontal line. Inset shows the variation of foverlap with ntr .

week ending 31 JANUARY 2014

out, however, this small long-range orientational order in the rotator phase of polyhedra does foreshadow the microscopic origin of their faster nucleation kinetics. To characterize orientational order in the growing nucleus, we calculate PCl 4 , the cubatic-order parameter of the greatest cluster for different values of ntr [see Fig. 2(b)]. In all cases, PCl 4 stays in the narrow range from 0.08 to 0.14 which is a small value but still an order of a magnitude larger than the value of 0.011 for the bulk liquid phase of all three polyhedra, indicative of incomplete orientational disorder in the solid nuclei. As shown in Fig. 2(b), PCl 4 is, however, smaller than the average P4 for the corresponding stable bulk-rotator phases (see [24]). To probe whether a distinguishable orientationally ordered cluster exists and whether it is correlated with the translationally ordered nucleus, we define an order parameter, nor , as the number of particles in the greatest cluster based on the rotationally invariant orientational order parameter, I 4 [37]. Akin to the translational order parameter, we define a local orientational order parameter I 4 ðiÞ for particle i (see [24]) and obtain nor with a procedure similar to that used to calculate ntr . We define as f overlap the fraction of particles in nor that are present in ntr . As shown in the inset of Fig. 2(b), f overlap ∼ 10%–20% at the precritical stages, increasing to ∼ 40% or higher at the critical stage for all cases. This shows that a significant degree of spatial coupling exists between orientational and translational order as the rotator-phase nucleates. To further characterize the spatial coupling between orientational and translational order, we plot in Figs. 3(a) and 3(b) the normalized density distributions of the local translational order [q6 ðiÞ] and local orientational order [I 4 ðiÞ] for the bulk isotropic and rotator phases of the polyhedra. In Fig. 3(a), we also show the q6 ðiÞ density distributions of the bulk isotropic and solid phases of HSs. All the distributions are plotted for a DSS value near 0.3. The isotropic phase q6 ðiÞ distributions of COs, TOs, RDs, and HSs are almost indistinguishable and exhibit significant overlap with those for the corresponding solid phases. This shows that, like in HSs, the isotropic phase of polyhedra contains small regions of high local translational order. But unlike HSs, which lack any degree of freedom for orientational order, the local orientational order in the bulk isotropic phase for the polyhedra spans a broad range of values between 0.1 and 0.4, around an average value of hI 4 ðiÞi ∼ 0.2. Importantly, these hI 4 ðiÞi values are much larger than the average I 4 values for the whole isotropic phase (∼0.02), indicative of spatially heterogeneous (short-range) orientational order. Note that COs show the highest amount of overlap between the isotropic phase and rotator phase I 4 ðiÞ, likely a reflection of their lower average orientational order of the bulk-rotator phase. Figure 3(d) shows that, similar to the regions of high local translational order [also present in HSs as shown in Fig. 3(c)], the regions of high local orientational order are small in size (correlation length) and

048301-3

PRL 112, 048301 (2014)

PHYSICAL REVIEW LETTERS

FIG. 3 (color online). Normalized probability density distribution of (a) q6 ðiÞ for the isotropic and solid (rotator) phases of COs, TOs, RDs, and HSs, and (b) I 4 ðiÞ for the isotropic and rotator phases of COs, TOs, and RDs. All configurations correspond to DSS ∼ 0.3. Snapshots for isotropic configurations of (c) HSs and (d) COs. Snapshots of CO configurations of (e) critical-sized (ntr ∼ 183) nuclei (boundary marked by dashed black line) and (f) a fully rotator phase. The snapshots only show selected particles: Translationally ordered particles [with q6 ðiÞ > 0.5] are green (light gray), orientationally ordered particles [with I 4 ðiÞ > 0.3] are red (medium gray), and translationally and orientationally ordered particles are blue (dark gray).

appear scattered throughout the system. Although these pervading orientationally ordered and translationally ordered “hot spots” do not always coincide, it is their spatial coupling what likely facilitates both the birth and growth [Fig. 3(e)] of the translationally ordered embryo, and eventually overtake the entire system in the rotator phase [Fig. 3(f)]. One possible metric of the coupling between local orientational and translational order is nboth defined as the number of particles in nor that are present in ntr (i.e., a measure of the overlap between the largest orientationally ordered cluster and the translationally ordered nucleus). If such a coupling is favorable to nucleation, then configurations with a larger nboth would tend to be associated with a larger probability to commit to the rotator phase (pB value)

week ending 31 JANUARY 2014

and, conversely, configurations with high pB values would tend to exhibit larger nboth values. As shown in Fig. 4(a), the average and maximum values of nboth indeed increase with pB . The inset of Fig. 4(a) shows that with increasing pB values, not only the average value of ntr increases but also the average value of nboth . These correlations of nboth with ntr and pB suggest that the nucleus would tend to grow in regions with stronger spatial coupling between localized fluctuations of orientational and translational order. Some direct evidence of the latter comes from visual examination of the critical cluster; Fig. 4(b) shows one example of how the cluster tends to grow in regions where it previously had both local orientational and translational order (compare snapshots I and IV). In this first study of solid-phase nucleation kinetics of polyhedral particles, disordered suspensions of COs, TOs, and RDs are predicted to form solids much faster than HSs, despite their similar rounded shape and overall phase behavior. Specifically, the rotator-phase nucleation barrier heights (and rates) for these polyhedra were found to be significantly lower (larger) than those for HSs at comparable DSS. Such differences may partially stem from differences in nuclei structure, which is hcp-like for the polyhedra while fcc-like for HSs. Our analysis also reveals a coupling between spatial fluctuations of orientational and translational order present in the isotropic phase of the polyhedra. This coupling can be seen as a positive feedback loop wherein the spontaneous local alignment of particles [16,17,38] (wherein neighbor particles tend to pack their flat facets parallel to each other) help steer particles toward positions with translational order; conversely, regions having established translational order (i.e.,

FIG. 4 (color online). (a) pB vs nboth for COs at P ¼ 4.1, TOs at P ¼ 2.8, and RDs at P ¼ 4.32. The inset shows the correlation between the average values of hnboth i and hntr i; (pB values increase from the bottom-left to the top-right). (b) Snapshots of critical (I and II) and postcritical (III and IV) nuclei of the same trajectory for TOs at P ¼ 2.8. Blue (dark gray) TOs are both translationally and orientationally ordered, red (medium gray) TOs are translationally ordered, and green (light gray) TOs are orientationally ordered. Snapshots II and IV only show blue (dark gray) TOs with snapshot IV also showing in light gray the newly added particles.

048301-4

PRL 112, 048301 (2014)

PHYSICAL REVIEW LETTERS

at the interface of the nucleus) in turn make fluctuations with high orientational order more prevalent. In the context of CNT (see Supplemental Material [24]), this coupling in fluctuations (absent in hard spheres) would be expected to produce two opposing effects on the nucleation rate: (i) Decrease the solid-liquid interfacial tension γ and, hence, the free-energy barrier ΔG, and (ii) reduce the attempt rate (prefactor) by temporarily “trapping” particles approaching the nucleus in nearby regions with correlated order. Overall, we conjecture that a catalytic effect may occur with other particle shapes forming rotator phases provided that local orientational order occurs and it couples synergistically with translational order (the “elongated spheres” of Ref. [39] would provide a counterexample). Some polyhedra could even be used as initiators to catalyze solid nucleation of spheres. This work was supported by the U.S. National Science Foundation, Grant No. CBET 1033349. The authors also thank U. Agarwal, Sai Pooja, and M. Kadhilkar for providing material for the codes used in this work, and A. Gantapara and M. Dijkstra for providing additional data on their Letter [18].

* [email protected] [1] P. Yi and G. C. Rutledge, Annu. Rev. Chem. Biomol. Eng. 3, 157 (2012). [2] D. Moroni, P. Rein ten Wolde, and P. G. Bolhuis, Phys. Rev. Lett. 94, 235703 (2005). [3] J. S. van Duijneveldt and D. Frenkel, J. Chem. Phys. 96, 4655 (1992). [4] P. R. ten Wolde, M. J. Ruiz-Montero, and D. Frenkel, Phys. Rev. Lett. 75, 2714 (1995). [5] P. R. ten Wolde, M. J. Ruiz-Montero, and D. Frenkel, J. Chem. Phys. 104, 9932 (1996). [6] C. Dellago, P. G. Bolhuis, F. S. Csajka, and D. Chandler, J. Chem. Phys. 108, 1964 (1998). [7] C. Dellago, P. G. Bolhuis, and D. Chandler, J. Chem. Phys. 110, 6617 (1999). [8] B. Peters and B. L. Trout, J. Chem. Phys. 125, 054108 (2006). [9] T. S. van Erp, D. Moroni, and P. G. Bolhuis, J. Chem. Phys. 118, 7762 (2003). [10] T. S. van Erp and P. G. Bolhuis, J. Comput. Phys. 205, 157 (2005). [11] R. J. Allen, P. B. Warren, and P. R. ten Wolde, Phys. Rev. Lett. 94, (2005). [12] R. J. Allen, D. Frenkel, and P. R. ten Wolde, J. Chem. Phys. 124, 024102 (2006).

week ending 31 JANUARY 2014

[13] G. M. Whitesides and M. Boncheva, Proc. Natl. Acad. Sci. U.S.A. 99, 4769 (2002). [14] S. C. Glotzer and M. J. Solomon, Nat. Mater. 6, 557 (2007). [15] C. Burda, X. Chen, R. Narayanan, and M. A. El-Sayed, Chem. Rev. 105, 1025 (2005). [16] U. Agarwal and F. A. Escobedo, Nat. Mater.10, 230 (2011). [17] P. F. Damasceno, M. Engel, and S. C. Glotzer, Science 337, 453 (2012). [18] A. P. Gantapara, J. de Graaf, R. van Roij, and M. Dijkstra, Phys. Rev. Lett. 111, 015501 (2013). [19] U. Agarwal and F. A. Escobedo, J. Chem. Phys. 137, 024905 (2012). [20] T. Schilling and D. Frenkel, Phys. Rev. Lett. 92, 085505 (2004). [21] A. Cuetos, R. van Roij, and M. Dijkstra, Soft Matter 4, 757 (2008). [22] A. Cuetos, E. Sanz, and M. Dijkstra, Faraday Discuss. 144, 253 (2009). [23] R. Ni, S. Belli, R. van Roij, and M. Dijkstra, Phys. Rev. Lett. 105, 088302 (2010). [24] See Supplemental Material at http://link.aps.org/ supplemental/10.1103/PhysRevLett.112.048301 for more details regarding simulation methods, order parameters, and FFS results. [25] C. Valeriani, E. Sanz, and D. Frenkel, J. Chem. Phys. 122, 194501 (2005). [26] E. Sanz, C. Valeriani, D. Frenkel, and M. Dijkstra, Phys. Rev. Lett. 99, 055501 (2007). [27] A. J. Page and R. P. Sear, Phys. Rev. Lett. 97, 065701 (2006). [28] C. Velez-Vega, E. E. Borrero, and F. A. Escobedo, J. Chem. Phys. 133, 105103 (2010). [29] S. L. Meadley and F. A. Escobedo, J. Chem. Phys. 137, 074109 (2012). [30] S. Auer and D. Frenkel, J. Chem. Phys. 120, 3015 (2004). [31] E. E. Borrero and F. A. Escobedo, J. Chem. Phys. 127, 164101 (2007). [32] S. Auer and D. Frenkel, Nature (London) 409, 1020 (2001). [33] J. Wedekind, R. Strey, and D. Reguera, J. Chem. Phys. 126, 134103 (2007). [34] E. Sanz and D. Marenduzzo, J. Chem. Phys. 132, 194102 (2010). [35] B. Cichocki and K. Hinsen, Physica (Amsterdam) 166A, 473 (1990). [36] L. Filion, M. Hermes, R. Ni, and M. Dijkstra, J. Chem. Phys. 133, 244115 (2010). [37] B. S. John, C. Juhlin, and F. A. Escobedo, J. Chem. Phys. 128, 044909 (2008). [38] G. V. Anders, N. K. Ahmed, D. Klotsa, M. Engel,, and S. C Glotzer, arXiv:1309.1187. [39] R. Ni and M. Dijkstra, J. Chem. Phys. 134, 034501 (2011).

048301-5